Fabrication of Laser Ablated Silver Nanoparticles in Bio-Polymeric Media
Metallic nanoparticle research is an attractive field in scientific studies due to the wide and varied ranges of potential and available applications, from biological to industrial areas. Recently, researchers have published various preparation methods of metal nanoparticles, including chemical and physical methods. Among the physical methods, the photo-irradiation synthesis method offers many advantages, such as space-selective fabrication. The pulsed laser ablation (PLA) method has also attracted attention due to its enormous potential in laser-based materials processing, such as nanocrystals; growth, solid thin film, surface cleaning, and microelectronic device fabrication. In addition, the PLA technique offers advantages in preparation methodology: (I) â€œsimple and cleanâ€? synthesis, (II) ambient conditions without extreme temperature and any special physical conditions such as pressure, and (III) formation of nanoparticles that may occur in both liquid and solid forms. However, the size effect using the PLA method in preparing metal nanoparticles has not been thoroughly investigated, although some approaches have considered the effect of PLA parameters and conditions on the size of metal nanoparticles [8, 9]. To date, no approach has been carried out on the preparation of Ag-NPs using gelatin as a stabilizer in the PLA method. In this paper, we used the PLA method to focus on the preparation of Ag-NPs from silver plate in water using gelatin as a stabilizer. The effect of the laser-pulsed repetition rate on size of Ag-NPs was studied.
Experimental Silver plate was used as a silver source and gelatin was used as a stabilizer for the fabrication of Ag-NPs. The silver plate was set in glass cell containing 20 mL of a fresh aqueous gelatin (1% wt.) solution, and the laser light was focused on the surface of the silver plate using a quartz lens (f = 25 cm). Laser ablation was carried out using a focused 532 nm laser light of a nanosecond Q-switched pulsed Nd:YAG laser (SL400/SL800 system) at 0.6 J/pulse for 15 min on different vessels for different repetition rates (e.g., 10, 20, 30, and 40 Hz).
Fig. 3 shows the TEM images of Ag-NPs in the colloidal solutions and their particle size distributions. The mean diameter and the standard deviation of Ag-NPs are also summarized in Table 1. The Ag-NPs with a mean diameter of less than 15 nm in all applied laser repetition rates; thus, it is clear that the size and particle size distribution of AgNPs significantly depend on applied laser repetition rates. The mean diameter and the particle size distributions of Ag-NPs increased as laser repetition rate becomes greater. The mean diameters of Ag-NPs prepared in 20 and 30 Hz were 11.3 and 13 nm, respectively.
Figure 2: UV-vis spectra of prepared Ag-NPs at different repetition rates.
Figure 1: The experimental set-up for preparation of Ag-NPs using the PLA method.
Results and discussion During the laser ablation of the silver target, the color of the solutions changed from colorless to light yellow, yellow, and finally light brown. Interestingly, the color of solution changed faster for the higher repetition rate than lower at the same intensity (0.6 J/pulse). The deeper the color was, the higher the concentration of Ag-NPs, which was confirmed using the UV-vis absorption spectra. Fig. 2 shows the UV-vis absorption spectra of silver colloids prepared using the PLA method in water with 532 nm laser light at different repetition rates. As shown in the UV-vis spectra, the SPR peak increases as the laser repetition rate increases, suggesting that the concentration of particles or the efficiency of particle formation increases at higher repetition rates. Repetition rate (Hz)
Mean diameter (nm)
Standard deviation (nm)
Table 1: The mean diameter of Ag-NPs prepared using the PLA method in aqueous solutions at different repetition rates (*without gelatin).
Figure 3: TEM images and particle size distributions of Ag-NPs prepared at different repetition rates; 10 (A), 20 (B), 30 (C), 40 (D), and 10 Hz (E, neat water).
Preparation of Ag-NPs in the gelatin matrix using the pulsed laser ablation method without any other reagents is simply possible. The particle size distributions of Ag-NPs at different repetition rates indicated that the smallest Ag-NPs were obtained at 10 Hz. Further experiments in this condition demonstrated that an increase in repetition rate caused an increase in particle size as well as size distributions. This work provides important advantages namely, simplicity, speed, and cleanness.
Project Leader 1:
Project Leader 2:
Dr. Majid Darroudi
Asso. Prof. Dr. Mansor Bin Ahmad
Department of Modern Sciences and Technologies, School of Medicine, Mashhad University of Medical Sciences, Mashhad, IRAN Email: firstname.lastname@example.org
Department of Chemistry Faculty of Science Universiti Putra Malaysia (UPM) Email: email@example.com